Hydrazone Crosslinked Polysaccharide-based Hydrogels for Soft Tissue Engineering
|Kustantaja||Tampere University of Technology|
|Tila||Julkaistu - 2 marraskuuta 2018|
|Nimi||Tampere University of Technology. Publication|
The main aim of this thesis was to ﬁnd an optimal hydrazone crosslinked hydrogel material for soft TE, especially for corneal and neural applications, and to characterize the hydrogels thoroughly using several methods. Diﬀerent polysaccharides, i.e., hyaluronan (HA), alginate (AL), and gellan gum (GG), and synthetic polymer polyvinyl alcohol (PVA) were modiﬁed with complementary reactive aldehyde- and hydrazide-groups to enable hydrazone crosslinking. Diﬀerent HA-PVA-, AL-PVA-, GG-HA-, and HA-HA-based hydrogels were fabricated by varying the gel parameters, i.e., the degree of substitution and molecular weight of the gel components, the ratio of components, and the polymer concentration of the hydrogels. The mechanical, rheological, swelling/deswelling, enzymatic degradation, and diﬀusion properties of the hydrogels were characterized. Since microstructure plays an essential role in the control of hydrogel properties, the microstructure of the hydrogels was also characterized using rheology- and diﬀusion (ﬂuorescence recovery after photobleaching, FRAP)-based methods. More precisely, the structural parameters, i.e., the mesh size, the average molecular weight of the polymer chain between neighboring crosslinks, and crosslinking density were evaluated. HA-HA-based hydrogels were intended for the regeneration of the corneal stroma. Therefore, their suitability for the delivery of human adipose stem cells (hASCs) was studied. The addition of collagen I, which is the main ECM component in the corneal stroma, was also tested. In addition, the suitability of HA-PVA- and AL-PVA-based hydrogels to serve as 3D supportive and biomimicking materials for human pluripotent stem cell-derived neuronal cells was tested. GG-HA-based hydrogels were not intended for any speciﬁc application, but their potential applicability as scaﬀold material for soft TE was tested in terms of their material properties.
Results showed that the fabrication of hydrazone crosslinked HA-PVA-, AL-PVA-, GGHA-, and HA-HA-based hydrogels from complementary reactive polymers was successful. The traditional crosslinking methods of GG were replaced with this method, and variable mechanical and physical properties were obtained by varying the gel parameters described earlier. These GG-HA-based hydrogels showed ionic nature of deswelling in the presence of cations. This means that the physical properties of the hydrogels can be controlled in diﬀerent solution environments. They also showed that their stiﬀness was similar to that of soft tissues at low strains. It should be noted that due to the non-linear elastic behavior of the hydrogels (and tissues), the stiﬀness was also presented as a function of strain, instead of only giving the second-order elastic constants. Overall, the properties and injectability of GG-HA-based hydrogels supported their potential use in soft TE.
For the fabrication of the HA-HA-based hydrogels, two diﬀerent types of aldehydeand hydrazide-modiﬁcations were tested. In order to promote hASC attachment and survival, collagen I was added to the hydrogel with better stability. This led to a reduced swelling ratio and increased hydrogel stiﬀness. Good optical properties (transparency and refractive index) were obtained with both gel types. However, even though all HAHA-based hydrogels showed good hASC survival directly after encapsulation, only in the collagen-containing hydrogel were cells with elongated morphology found. Furthermore, the cornea organ culture model suggested that these hydrogels could be used as injectable cell delivery vehicles to corneal stromal defects. The biodegradability of HA, the favorable characteristics of hydrazone crosslinking, and the results described above all support the use of these hydrogels as potential materials for hASC delivery in the treatment of corneal stromal defects.
To the best of our knowledge, this is the ﬁrst time that the polymerization and properties of the hydrazone crosslinked AL-PVA hydrogel has been reported. The AL-PVA hydrogel, together with HA-PVA-based hydrogels, were fabricated and their properties were changed by varying the gel parameters described earlier. When the eﬀect of the gel parameters on the growth of human pluripotent stem cell-derived neuronal cells was tested, the results showed that the most supportive hydrogels had brain-mimicking mechanical properties at low strains, and that they contained a high molecular weight HA component. In addition, the lowering of the polymer concentration (softer hydrogels) resulted in enhanced neuronal growth. The AL-PVA hydrogel was shown to be similarly supportive. The neuronal spreading and 3D network formation were enhanced inside the softest hydrogels. Based on these results, the HA-PVA- and AL-PVA-based hydrogels were considered to be potential supportive biomaterials for 3D neural cell cultures.
The microstructures of the previously described hydrogels were evaluated thoroughly for the ﬁrst time using rheology- and FRAP-based methods. With these methods, the microstructure can be determined from wet samples, with no need to use destructive drying. The obtained results supported each other, i.e., diﬀusivity decreased when larger dextran sizes (500 kDa and 2000 kDa) were used, and those molecule sizes were equivalent to the mesh sizes of hydrogels (15 nm to 47 nm) determined by the rheological method. This size range allows the transportation of small molecules, peptides, and most of the proteins. The results also showed a proportionality between the structural parameters and storage moduli (and second order elastic constants). In summary, the results showed that hydrazone crosslinking oﬀers an easy way to produce polysaccharide-based hydrogels with tunable properties that are suitable for soft TE applications.